Abstract
We investigate the possibility of achieving the roomtemperature superconductivity in hydrogen sulfide (H_{3}S) through increasing external pressure, a path previously widely used to reach metallization and superconducting state in novel hydrogenrich materials. The electronic properties and superconductivity of H_{3}S in the pressure range of 250–500 GPa are determined by the firstprinciples calculations. The metallic character of a bodycentered cubic Im\(\overline{{\bf{3}}}\)m structure is found over the whole studied pressure. Moreover, the absence of imaginary frequency in phonon spectrum implies that this structure is dynamically stable. Furthermore, our calculations conducted within the framework of the Eliashberg formalism indicate that H_{3}S in the range of the extremely high pressures is a conventional strongcoupling superconductor with a high superconducting critical temperature, however, the maximum critical temperature does not exceed the value of 203 K.
Introduction
The recent breakthrough theoretical calculations^{1, 2} confirmed by spectacular experimental reports of the superconductivity in hydrogen sulfide, with the record high critical temperature equals to 203 K at pressure closed to 150 GPa^{3,4,5}, open the door to achieving the roomtemperature superconductivity in the compressed hydrogenrich materials^{6,7,8} or in the pristine metallic hydrogen^{9,10,11,12}. In contrast to the cuprates^{13, 14}, where the mechanism responsible for the superconducting state is still debated^{15,16,17,18,19,20,21,22}, the phononmediated pairing scenario is generally accepted in the case of H_{3}S^{23,24,25,26,27} due to the observed of a large isotope effect which convincingly suggest that hydrogen sulfide is a conventional superconductor^{3, 4}. Therefore, in the theoretical papers^{28,29,30,31,32}, the superconducting properties of hydrogen sulfide are studied in the framework of the meanfield BardeenCooperSchrieffer (BCS) theory^{33, 34}, or more precisely using the MigdalEliashberg (ME) approach^{35,36,37}. For the crystal structures of highT_{ C } hydrides, the highpressure xray diffraction experiments combined with the electrical resistance measurements^{5, 38} confirm that H_{3}S takes a bodycentered cubic \(Im\overline{3}m\) structure, which is certainly stable above 180 GPa^{2, 39}. The pressuretemperature phase diagram of solid hydrogen sulfide, determined on the base of a sharp falls to zero in resistivity with cooling, shows increase of T _{ C } from 95 to 203 K in the range of pressure from 110 to 155 GPa^{3, 5} and, then, further increasing of compression causes a linear decrease of critical temperature to 170 K at 225 GPa^{3}. There arises the natural question, whether under the influence of the high pressure is it possible to obtain the superconducting state with the value of the critical temperature even higher than 203 K in the case of H_{3}S compound. Below, we present the results of the ab initio calculations, which conclude that T _{ C } does not exceed the value of 203 K, while the range of the pressure from 250 to 500 GPa is adopted.
Computational details
The searches for the stable high pressure structures of H_{3}S system were performed through the evolutionary algorithm implemented in the USPEX code^{40, 41}, which has been applied successfully to a number of compressed systems containing hydrogen^{42, 43}. The computed enthalpy differences relative to the Cccm structure (H − H _{ Cccm }) as a function of pressure for the selected crystal structures are presented in Fig. 1. It can be clearly seen that at low pressure (below 110 GPa) the lowest value of enthalpy corresponds to the orthorhombic Cccm structure and the hexagonal R3m structure has the most stable lattice between 110 and 180 GPa. Then, a cubic \(Im\overline{3}m\) structure becomes favorable above 180 GPa. This structure is characterized by two S atoms located at a simple body centered cubic lattice and H atom situated midway between the two S atoms (see the inset in Fig. 1). Let us emphasize that for the low pressures our results agree well with the data reported by Duan et al.^{2}. Moreover, for H_{3}S the secondorder structural phase transition from R3m to \(Im\overline{3}m\) is also experimentally observed but for a slightly lower pressure (~150 GPa)^{5, 44}. It should be underlined that over 450 various structures were studied, wherein in any case was obtained enthalpy lower than \({H}_{Im\overline{3}m}\) in the range of pressures from 250 to 500 GPa. Due to the above fact in this study the critical temperature and the other thermodynamic parameters of the superconducting state of H_{3}S are calculated only for the structure \(Im\overline{3}m\). Figure 2 presents the curve of the volumepressure type. This curve can be reproduced with the help of the thirdorder BirchMurnaghan equation: \(p(V)=\frac{3}{2}{B}_{0}[{({V}_{0}/V)}^{\mathrm{7/3}}{({V}_{0}/V)}^{\mathrm{5/3}}]\,\{1+\frac{3}{4}({B}_{0}^{^{\prime} }4)[{({V}_{0}/V)}^{\mathrm{2/3}}1]\}\), where B _{0} = 129.8 GPa, \({V}_{0}=158.4\,{{\rm{a}}}_{0}^{3}\), and \({B}_{0}^{^{\prime} }=3.6\) ^{39}.
The characteristics of the electron structure, the phonon structure, and the electronphonon interaction was made in the framework of the QuantumESPRESSO package^{45}. The calculations were conducted basing on the densityfunctional methods using the PWSCF code^{45,46,47}. The Vanderbilttype ultrasoft pseudopotentials for S and H atoms were employed with the kinetic energy cutoff equal to 80 Ry. The phonon calculations were performed for 32 × 32 × 32 MonkhorstPack kmesh with the Gaussian smearing of 0.03 Ry. The electronphonon coupling matrices were computed using 8 × 8 × 8 qgrid. The superconducting transition temperature (T _{ C }) can be in a simple way estimated using the AllenDynes modified McMillan equation^{48}:
where k _{ B } = 0.0862 meV/K (the Boltzmann constant), f _{1} and f _{2} are the correction functions:
The quantity ω _{2} represents the second moment of the normalized weight function:
and ω _{ln} is the logarithmic average of the phonon frequencies:
More sophisticated calculations can be conducted within the framework of the Eliashberg formalism, which allows a more accurately description of the superconducting state in strongcoupling systems^{31, 32}. The Eliashberg equations for the superconducting order parameter function \({\phi }_{m}\equiv \phi \,(i{\omega }_{m})\) and the electron mass renormalization function \({Z}_{m}\equiv Z\,(i{\omega }_{m})\) written in the imaginaryaxis formulation take the following form refs 36 and 49:
and
where the pairing kernel for the electronphonon interaction is given by:
Symbols \({\mu }^{\ast }\) and θ denote the Coulomb pseudopotential and the Heaviside function with cutoff frequency ω _{ c } equal to three times the maximum phonon frequency (ω _{ D }). The α ^{2} F(ω) functions, called the Eliashberg functions, for H_{3}S system were calculated using the density functional perturbation theory and the planewave pseudopotential method, as implemented in the QuantumEspresso package^{45}:
with
where \(\rho \,({\varepsilon }_{F})\) denotes the density of states at the Fermi energy, ω _{ q ν } determines the values of the phonon energies, and γ _{ q ν } represents the phonon linewidth. The electronphonon coefficients are given by g _{ q ν } (k, i, j) and \({\varepsilon }_{{\bf{k}},i}\) is the electron band energy.
Results and Discussion
To investigate the electronic properties of H_{3}S at \(p\in \langle 250,500\rangle \,{\rm{GPa}}\), we calculate the electronic band structure and density of states (DOS). The Fermi surface of H_{3}S at 250 and 500 GPa is shown in Fig. 3. It is formed by five different Fermi surfaces calculated in the bcc Brillouin zone^{50}. As has been previously reported by Bianconi and Jarlborg, the red small Fermi surface centered at the Γpoint and covering the surfaces #1 and #2, appears above 95 GPa with the change of the Fermi surface topology. This change of the Fermi surface topology is called a L1 Lifshitz transition for a new appearing Fermi surface spot and occurs where the bands at the Γpoint cross the chemical potential. The L2 Lifshitz transition for neck disrupting occurs around 180–200 GPa and is connected with appearing of the small tubular necks in the Fermi surface (in particular in the surface #4)^{50, 51}.
The results presented in Fig. 4 clearly show that \(Im\overline{3}m\) structure is a good metal with a large DOS at the Fermi level (0.418–0.511 states/eV/f.u.). This is in a good agreement with the previous theoretical and experimental results obtained for the lower pressure^{3,4,5, 52}. The metallic behavior of this system indicates that \(Im\overline{3}m\) phase might be superconducting above 250 GPa.
In order to investigate the superconductivity of H_{3}S, the phonon band structures, the phonon density of states (PhDOS) and the Eliashberg spectral functions together with the electronphonon integrals \(\lambda (\omega )=2{\int }_{0}^{\omega }\,d\omega {\alpha }^{2}F(\omega )/\omega \) were carried out. As shown in Fig. 5 there is no imaginary frequency to be found in the whole Brillouin zone, confirming that \(Im\overline{3}m\) is a dynamically stable structure. In the case of the pressure of 250 GPa, the clearly separated lines respectively associated with the lowenergy vibrations of sulfur (\(\omega \in \langle \mathrm{0,76.4}\rangle \,{\rm{meV}}\)) and the highenergy vibrations of hydrogen (\(\omega \in \langle \mathrm{95.2,256.7}\rangle \,{\rm{meV}}\)) can be noticed in the phonon dispersive relation. Such fact directly translates into the shape of the function of the phonon density of states, which consists of two parts separated by the gap of the energy (about 19 meV). On the basis of the diagram related to the spectral function it can be seen that the contribution to the electronphonon coupling constant comes mainly from hydrogen, and is equal approximately to 79%. At the pressure of 350 GPa, the maximum energy of the hydrogen vibrations becomes larger and equals to 308.7 meV. Still visible is the division of functions of the phonon density of states on the part related to sulfur and hydrogen. However, the energy gap width decreases, and is approximately 14 meV. The contribution of hydrogen to the electronphonon coupling constant is still dominating (around 66%). The increase of the pressure by the further 150 GPa causes the renewed increase in the maximum vibration energy of hydrogen \({[{\omega }_{D}]}_{500{\rm{GPa}}}/{[{\omega }_{D}]}_{350{\rm{GPa}}}=1.179\). However, the division of the phonon density of states on the portion derived from sulfur and hydrogen is galling. The disappearance of the sulfurhydrogen separation results also in the slight increase of the value of the electronphonon coupling constant in the range of the lower frequencies \({\lambda }_{500{\rm{GPa}}}(\omega =120\,{\rm{meV}})/{\lambda }_{350{\rm{GPa}}}(\omega =120\,{\rm{meV}})=1.29\). Above the pressure of 500 GPa we found the imaginary (negative) phonon frequencies which is an indication of the structural instability. This is one of the reason why we have limited our calculations to this range of pressures, the second one is that higher pressures are far beyond the ability of the experiment. In light of the latest results on the metallization of hydrogen^{53}, compression up to 500 GPa is possible to achieve in laboratory.
Figure 6 ilustrates the pressure dependence of the superconducting critical temperature. Close and open circles corresponds to the experimental results presented by Drozdov et al.^{3} and Einaga et al.^{5}, respectively. The red dashed lines drawn by eye represents the trend of the experimental data above 150 GPa and great combine together with the theoretical range of T _{ C } calculated for the high pressures. These theoretical results were obtained using the Eliashberg equations and the following relation: \({{\rm{\Delta }}}_{m=1}(T={T}_{C})=0\), where the order parameter is defined as \({{\rm{\Delta }}}_{m=1}={\phi }_{m=1}/{Z}_{m=1}\). The commonly accepted value of the Coulomb pseudopotential \({\mu }^{\ast }=0.13\) was adopted, the exact results of T _{ C } are collected in Table 1. The error bars indicate the value range of T _{ C } with \({\mu }^{\ast }\in \langle 0.11,0.15\rangle \). The obtained results show that T _{ C } decreases from 164 to 129 K in the range of pressure from 250 to 350 GPa. Then above 350 GPa the superconducting critical temperature starts increasing. This is a promising result, however in the range of the pressure from 350 to 500 GPa the critical temperature does not exceed the value of 203 K. This can be explained by the unfavorable, and simultaneously weak, variation of the electronphonon coupling constant and the logarithmic phonon frequency (the insert in Fig. 6). From the conducted ab initio calculations comes the conclusion that this is caused by the small or unfavorable influence of the pressure on the electron density of states and the electronphonon matrix elements. It can be, however, noticed that the value of T _{ C } in the range of the very high pressures is relatively high and does not drop below 120 K. We did not study the critical temperature under extreme pressures because beyond 500 GPa the H_{3}S structure loses the dynamical stability.
Then, by using the analytical continuation^{37, 49}, we determine the superconducting energy gap Δ(0) and the dimensionless ratio 2Δ(0)/T _{ C } which in the BCS theory takes the constant value 3.53. As we can see in Table 1, the obtained results significantly exceed the value of BCS predictions. This is connected with the strongcoupling and retardation effects, which in the framework of the Eliashberg formalism are not neglected. During the preparation of this manuscript, a superconducting energy gap of H_{3}S compressed to 150 GPa was experimentally found (2Δ = 73 meV)^{54}. Taking into account this result and the previously determined value of T _{ C } at this same pressure (203 K)^{3} we can evidence that 2Δ/k _{ B } T _{ C } = 4.17 is surprisingly close to our predictions for higher pressures. The above fact proves the correctness of our calculations.
Conclusions
In this paper we showed that H_{3}S exhibits the superconducting properties in the range of the very high pressures (250–500 GPa), however, the critical temperature does not exceed the value of 203 K. The obtained result is related to the weak and unfavorable volatility of the electronphonon coupling constant and the logarithmic phonon frequency. From the microscopic point of view, this results from the small or unfavorable influence of the pressure on the value of the electron density of states at the Fermi surface and the electronphonon matrix elements. According to the above, it can be seen that the increase of the pressure alone is not sufficient to obtain the superconducting state in H_{3}S at the room temperature. It is possible that the better method to achieve this goal is the appropriate partial atomic substitution of S atoms by other atoms. Interesting theoretical results were obtained by Ge et al. in the paper^{55}, where the increase of the Psubstitution rate causes the increase of the DOS, the phonon linewidths and the electronphonon coupling constant. Finally, T _{ C } = 280 K for H_{3}S_{0.925}P_{0.075} at 250 GPa.
References
 1.
Li, Y., Hao, J., Liu, H., Li, Y. & Ma, Y. The metallization and superconductivity of dense hydrogen sulfide. J. Chem. Phys. 140, 174712 (2014).
 2.
Duan, D. et al. Pressureinduced metallization of dense (H_{2}S)_{2}H_{2} with highT_{ C } superconductivity. Sci. Rep. 4, 6968 (2014).
 3.
Drozdov, A. P., Eremets, M. I., Troyan, I. A., Ksenofontov, V. & Shylin, S. I. Conventional superconductivity at 203 kelvin at high pressures in the sulfur hydride system. Nature 525, 73 (2015).
 4.
Troyan, I. et al. Observation of superconductivity in hydrogen sulfide from nuclear resonant scattering. Science 351, 1303 (2016).
 5.
Einaga, M. et al. Crystal structure of the superconducting phase of sulfur hydride. Nat. Phys. 12, 835–838 (2016).
 6.
Ashcroft, N. W. Hydrogen dominant metallic alloys: high temperature superconductors? Phys. Rev. Lett. 92, 187002 (2004).
 7.
Wang, H., Tse, J. S., Tanaka, K., Iitaka, T. & Ma, Y. Superconductive sodalitelike clathrate calcium hydride at high pressures. Proc. Natl. Acad. Sci. USA 109, 6463 (2012).
 8.
Feng, X., Zhang, J., Gao, G., Liu, H. & Wang, H. Compressed sodalitelike MgH_{6} as a potential hightemperature superconductor. RSC Adv. 5, 59292–59296 (2015).
 9.
Ashcroft, N. W. Metallic hydrogen: a hightemperature superconductor? Phys. Rev. Lett. 21, 1748 (1968).
 10.
Cudazzo, P. et al. Ab initio description of hightemperature superconductivity in dense molecular hydrogen. Phys. Rev. Lett. 100, 257001 (2008).
 11.
McMahon, J. M. & Ceperley, D. M. Groundstate structures of atomic metallic hydrogen. Phys. Rev. Lett. 106, 165302 (2011).
 12.
McMahon, J. M. & Ceperley, D. M. Hightemperature superconductivity in atomic metallic hydrogen. Phys. Rev. B 84, 144515 (2011).
 13.
Bednorz, J. G. & Müller, K. A. Possible high T_{ C } superconductivity in the BaLaCuO system. Z. Phys. B 64, 189 (1986).
 14.
Bednorz, J. G. & Müller, K. A. Perovskitetype oxides  the new approach to highT_{ C } superconductivity. Rev. Mod. Phys. 60, 585 (1988).
 15.
Emery, V. J. Theory of highT_{C} superconductivity in oxides. Phys. Rev. Lett. 58, 2794 (1987).
 16.
Dagotto, E. Correlated electrons in hightemperature superconductors. Rev. Mod. Phys. 66, 763 (1994).
 17.
Damascelli, A., Hussain, Z. & Shen, Z. X. Angleresolved photoemission studies of the cuprate superconductors. Rev. Mod. Phys. 75, 473 (2003).
 18.
Krzyzosiak, M., Gonczarek, R., Gonczarek, A. & Jacak, L. Applications of the conformal transformation method in studies of composed superconducting systems. Front. Phys. 11, 117407 (2016).
 19.
Cuk, T. et al. A review of electronphonon coupling seen in the highT_{C} superconductors by angleresolved photoemission studies (ARPES). Phys. Status Solidi B 242, 11 (2005).
 20.
Tarasewicz, P. & Baran, D. Extension of the Fröhlich method to 4fermion interactions. Phys. Rev. B 73, 094524 (2006).
 21.
Szczęśniak, R. Pairing mechanism for the highT_{ C } superconductivity: symmetries and thermodynamic properties. PloS One 7, e31873 (2012).
 22.
Szczęśniak, R. & Durajski, A. P. Anisotropy of the gap parameter in the holedoped cuprates. Supercond. Sci. Technol. 27, 125004 (2014).
 23.
Mazin, I. I. Superconductivity: Extraordinarily conventional. Nature 525, 40 (2016).
 24.
Bernstein, N., Hellberg, C. S., Johannes, M. D., Mazin, I. I. & Mehl, M. J. What superconducts in sulfur hydrides under pressure and why. Phys. Rev. B 91, 060511 (2015).
 25.
Ortenzi, L., Cappelluti, E. & Pietronero, L. Band structure and electronphonon coupling in H_{3}S: A tightbinding model. Phys. Rev. B 94, 064507 (2016).
 26.
Sano, W., Koretsune, T., Tadano, T., Akashi, R. & Arita, R. Effect of van Hove singularities on highT_{ C } superconductivity in H_{3}S. Phys. Rev. B 93, 094525 (2016).
 27.
Gor’kov, L. P. & Kresin, V. Z. Pressure and highT_{ C } superconductivity in sulfur hydrides. Sci. Rep. 6, 25608 (2016).
 28.
Errea, I. et al. Highpressure hydrogen sulfide from first principles: A strongly anharmonic phononmediated superconductor. Phys. Rev. Lett. 114, 157004 (2015).
 29.
Durajski, A. P., Szczęśniak, R. & Li, Y. NonBCS thermodynamic properties of H_{2}S superconductor. Physica C 515, 1 (2015).
 30.
FloresLivas, A. J., Sanna, A. & Gross, E. K. U. High temperature superconductivity in sulfur and selenium hydrides at high pressure. Eur. Phys. J. B 89, 1 (2016).
 31.
Durajski, A. P., Szczęśniak, R. & Pietronero, L. Hightemperature study of superconducting hydrogen and deuterium sulfide. Ann. Phys. (Berlin) 528, 358 (2016).
 32.
Durajski, A. Quantitative analysis of nonadiabatic effects in dense H_{3}S and PH_{3} superconductors. Sci. Rep. 6, 38570 (2016).
 33.
Bardeen, J., Cooper, L. N. & Schrieffer, J. R. Microscopic theory of superconductivity. Phys. Rev. 106, 162 (1957).
 34.
Bardeen, J., Cooper, L. N. & Schrieffer, J. R. Theory of superconductivity. Phys. Rev. 108, 1175 (1957).
 35.
Migdal, A. B. Interaction between electrons and lattice vibrations in a normal metal. Soviet Physics JETP 34, 996 (1958).
 36.
Eliashberg, G. M. Interactions between electrons and lattice vibrations in a superconductor. Soviet Physics JETP 11, 696 (1960).
 37.
Carbotte, J. P. Properties of bosonexchange superconductors. Rev. Mod. Phys. 62, 1027 (1990).
 38.
Li, Y. et al. Dissociation products and structures of solid H_{2}S at strong compression. Phys. Rev. B 93, 020103 (2016).
 39.
Errea, I. et al. Quantum hydrogenbond symmetrization in the superconducting hydrogen sulfide system. Nature 532, 81 (2016).
 40.
Oganov, A. R. & Glass, C. W. Crystal structure prediction using ab initio evolutionary techniques: Principles and applications. J. Chem. Phys Physics 124, 244704 (2006).
 41.
Glass, C. W., Oganov, A. R. & Hansen, N. USPEXevolutionary crystal structure prediction. Comput. Phys. Commun. 175, 713 (2006).
 42.
Esfahani, M. M. D. et al. Superconductivity of novel tin hydrides (Sn_{ n }H_{ m }) under pressure. Sci. Rep. 6, 22873 (2016).
 43.
Liu, Y. X. et al. Structures and properties of osmium hydrides under pressure from first principle calculation. J. Phys. Chem. C 119, 15905–15911 (2015).
 44.
Einaga, M. et al. Twoyear progress in experimental investigation on hightemperature superconductivity of sulfur hydride. Jpn. J. Appl. Phys. 56, 05FA13 (2017).
 45.
Giannozzi, P. et al. QUANTUM ESPRESSO: a modular and opensource software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
 46.
Hohenberg, P. & Kohn, W. Inhomogeneous electron gas. Phys. Rev. 136, B864 (1964).
 47.
Kohn, W. & Sham, L. J. Selfconsistent equations including exchange and correlation effects. Phys. Rev. 140, A1133 (1965).
 48.
Allen, P. B. & Dynes, R. C. Transition temperature of strongcoupled superconductors reanalyzed. Phys. Rev. B 12, 905 (1975).
 49.
Marsiglio, F., Schossmann, M. & Carbotte, J. P. Iterative analytic continuation of the electron selfenergy to the real axis. Phys. Rev. B 37, 4965 (1988).
 50.
Bianconi, A. & Jarlborg, T. Superconductivity above the lowest earth temperature in pressurized sulfur hydride. Europhys. Lett. 112, 37001 (2015).
 51.
Jarlborg, T. & Bianconi, A. Breakdown of the migdal approximation at lifshitz transitions with giant zeropoint motion in H_{3}S superconductor. Sci. Rep. 6, 24816 (2016).
 52.
Akashi, R., Kawamura, M., Tsuneyuki, S., Nomura, Y. & Arita, R. Firstprinciples study of the pressure and crystalstructure dependences of the superconducting transition temperature in compressed sulfur hydrides. Phys. Rev. B 91, 224513 (2015).
 53.
Dias, R. P. & Silvera, I. F. Observation of the wignerhuntington transition to metallic hydrogen. Science 355, 715–718 (2017).
 54.
Capitani, F. et al. Spectroscopy of H_{3}S: evidence of a new energy scale for superconductivity. arXiv:1612.06732v2 (2016).
 55.
Ge, Y., Zhang, F. & Yao, Y. Firstprinciples demonstration of superconductivity at 280 K in hydrogen sulfide with low phosphorus substitution. Phys. Rev. B 93, 224513 (2016).
 56.
Fan, F., Papaconstantopoulos, D. A., Mehl, M. J. & Klein, B. M. Theory of the superconducting state. I. the ground state at the absolute zero of temperature. J. Phys. Chem. Solids 99, 105 (2016).
Acknowledgements
A.P.D. gratefully acknowledges financial support from the Częstochowa University of Technology under Grant No. BS/MN203301/2017.
Author information
Affiliations
Contributions
A. P. Durajski designed and carried out the abinitio calculations, collected data and drafted the final version of the manuscript. R. Szczęśniak wrote the part of the code for numerical calculations and participated in writing the manuscript. All authors reviewed the manuscript.
Corresponding author
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Durajski, A.P., Szczęśniak, R. Firstprinciples study of superconducting hydrogen sulfide at pressure up to 500 GPa. Sci Rep 7, 4473 (2017). https://doi.org/10.1038/s41598017047145
Received:
Accepted:
Published:
Further reading

Thermodynamic Properties of the Superconducting State in Metallic Hydrogen: Electronic Correlations, Nonconventional ElectronPhonon Couplings and the Anharmonic Effects
Journal of Superconductivity and Novel Magnetism (2021)

From LaH10 to room–temperature superconductors
Scientific Reports (2020)

RealTime Evolution of the Electron Clouds of Transition Metal Ions: Possible ElectronPairing Medium in Unconventional HighTemperature Superconductors
Journal of Superconductivity and Novel Magnetism (2019)

Unusual sulfur isotope effect and extremely high critical temperature in H3S superconductor
Scientific Reports (2018)

Anomalously high value of Coulomb pseudopotential for the H5S2 superconductor
Scientific Reports (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.